FEM Modeling of a 3D Printed Carbon Fiber Pylon

 Adrian Preston
 10 months ago
 Views:
Transcription
1 FEM Modeling of a 3D Printed Carbon Fiber Pylon I. López G.*, B. Chiné, and J.L. León S. Costa Rica Institute of Technology, School of Materials Science and Engineering, Cartago, Costa Rica *Corresponding author: P.O. Box , Cartago, Costa Rica, Abstract: The evolution of specific three dimensional (3D) printing fabrication technologies has developed the capability to fabricate functional parts in several fields of the engineering. The aim of this study is to evaluate the elastic properties of 3D printed carbon fiber pylon under compression stress and compare them with experimental data, in order to estimate its properties and allow mechanical analysis by computational tools. 3D printed polymeric samples are fabricated through a continuous fiber fabrication (CFF) process. The principal elastic E Z and E y are obtained by developing experimental tests under ASTM D695 standard. The shear is computed from the composite theory, by managing specific values of the Poisson ratio. The modeling work in COMSOL Multiphysics 5.2a is developed under static conditions, using the Solid Mechanics module. The CAD geometries of the printed pylon are created in Solid Works and then imported to COMSOL. Two different CAD models are designed: the first one is a laminated specimen, while the second one is a solid orthotropic material. Appropriate boundary conditions are set in order to model the experimental condition. Then, by developing the simulation work with COMSOL Multiphysics, a simple mechanical performance of the pylon is simulated. Keywords: carbon fiber pylon, solid mechanics, compression stress, FEM. 3D printing technologies, provides the possibility to improve the mechanical properties of the material used in additive manufacture. However, the implementation of functional part fabricated by 3D printing technologies is difficult, because several factors affect the mechanical properties of these parts (Domingo Espin et al., 2015; Wu et al., 2015). To ensure the mechanic resistance of 3D printed parts, it is necessary to evaluate the mechanical properties of the material under enduse mechanism loads (DomingoEspin, et al, 2015; Sutradhar et al., 2014). The mechanical behavior of 3D printed parts has been studied by FEM (DomingoEspin et al., 2015; Sutradhar et al., 2014; Góski et al., 2015; Sayre, 2014). DomingoEspin et al (2015) concludes what the if the polymeric material does not exceed the yield stress, it can be considered as isotropic. But, to evaluate a FEA model of 3D printed FRP parts is necessary to assume a no homogeneous material, because the reinforce fiber produces specifics effect on the mechanical behavior (Mallick, 2008). In this paper we develop an experimental work to evaluate the compression properties of 3D printed carbon reinforced parts and a successive computational work to simulate the mechanical performance of the 3D printed prosthetic pylon of Fig. 1. In the next sections, a brief introduction concerning the property of the pylon is given at the beginning, followed by the description of the experimental and 1. Introduction Additive Manufacture Technology provides the possibility to work with many polymers, although a few ones can be used as functional parts in engineering applications, because these materials are not enough resistant for a final product (DomingoEspin et al., 2015). Improvements on Fused Filament Fabrication (FFF) technology have allowed the possibility to fabricate parts by continuous fiber reinforced polymers and additive manufacture technologies. Another process like the CBAM has the possibility to create parts, based on thin carbon layers and polymers. The fabrication of fiber reinforced polymer (FRP), by Figure 1. Schematic of the prosthetic pylon.
2 computational works. Finally, the results obtained in our work are presented and analyzed. 2. Theory The direction of the reinforce fiber is the principal factor affecting the mechanical properties of reinforced parts (Mallick, 2008). It is important to define bidirectional reinforced architecture on fabricated parts to improve the performance of parts in two directions. In order to study the mechanical behavior of 3D printed reinforced parts by FEM, it is important to consider the orthotropic characteristic of the reinforced polymers. In some cases, it could be necessary to determinate the nine engineering elastic constants of materials. However, fabrication process can configure bidirectional reinforced on the xz plane, where the z orientation is normal to the figure plane in Fig. 2. This configuration produces a mechanical equivalence on z and x direction (Mallick, 2008; DomingoEspin et al., 2015). To determinate some To evaluate the bidirectional reinforce material, at least two Young s (E ij), two Poisson s ratio (ʋ ij) and two shears (G ij) must be found (Mallick, P. 2008). 3. Experimental work As our focus is the mechanical compression of reinforced polymer, three different samples are evaluated under compression stresses. Sample dimensions are 12x12x24 mm, fabricated with the A and B orientations of Fig. 3, with 100% infill, mm of layer thickness and concentric fiber reinforced on approximately 30% of layers. Supplier configurations of temperature and velocity of the print process are used. Following the ASTM D695 standard for compression properties of reinforced polymers, we test three different specimens with the A and B orientations of Fig. 3. Figure 3. Sample orientations evaluated. εx εy εz γyz γxz γzy Figure 2. Example of a layer configuration of 3D reinforced part. mechanical properties that cannot be measured by experimental test, it is possible to use analytical and mathematical approximations under the mixture law (Mallick, 2008). Orthotropic materials are defined by three mutually perpendicular symmetry planes. By analyzing the mechanical behavior of materials under elastic strain, the mechanical performance is defined by the compliance matrix, which is written in terms of Young s, Poisson s ratio and shear by (1) (DomingoEspin et al., 2015): 1/Ex ʋxy/ex ʋxz/ex ʋxy/ex 1/Ey ʋyz/ex ʋxz/ex ʋyz/e 1/Ez = /Gyz /Gxz /Gxy * ( 1 ) σx σy σz τyz τxz τzy Mechanical tests in A and B direction provide the E z and E y of the material. Then, it is possible to determinate the shear and Poisson s ratio by the mathematical approximations (2) and (3): G xy = E xx 2(1+ʋ xy ) ʋ xy = ε xx ε yy (2) (3) Compression tests follow the ASTM D695 standard requirements. We use a Tinius Olsen equipment with a load of 50 kn and a velocity load of 1.3mm/seg. The Young s is computed by the slope of the linear plot in the elastic region. 4. Computational work Using COMSOL Multiphysics 5.2a, we develop a stationary study of the 3D pylon using the Structural Mechanics module and analyzing only the linear elastic behavior. A first FEM model assumes an
3 isotropic material while a second one considers a laminated material fabricated by polymer matrix and thin fiber layers of carbon fiber, with isotropic properties. Finally, a third model analyses a solid orthotropic material with properties of an orthotropic composite material. In order to simulate the experimental compression test, we prescribe displacements equal to zero in the z direction for the lower boundary of the sample part (Fig. 4). Also, we use a fix constrain in the upper part of the disc base. We apply a force of approximately N in the z direction on the upper side of the sample. With this total force, we should simulate the experimental yield stress of the material, which is 42 MPa approximately. Table 1: Estimated material properties of the isotropic material. Young Ey Ez = Ex Magnitude [GPa] [GPa] ʋyz = ʋxz 0.4 ʋxy 0.4 Gxy Gyz= Gxz [GPa] [GPa] Table 2: Polymer matrix and carbon fiber (C.F.) mechanical properties. Figure 4. Boundary constraints. Initially, an isotropic model material is simulated with a Young s module equal to E z (Table 1). Then, a second CAD laminated material model is evaluated with two different properties, calculated by the mixture law, given the volume of each constituent material (30% carbon fiber, approximately). In this case, polymer matrix and carbon fiber were defined as isotropic materials. The material properties of the polymer matrix have been obtained by the mechanical test, while the carbon fiber properties have been deduced by the mixture law (Table 2). A second model for the laminated material simulates a reinforced material by thin layers. Hence, we use the mixture law to define the Young of matrix and fiber components. In the model each material is defined as isotropic. A third model with an orthotropic material has been developed using the orthotropic constants obtained by experimental and mathematical methods, which are given also in Table 1. Using COMSOL Multhiphysics 5.2a we simulate the mechanical tests, using experimental (E ij) and analytical (ʋ ij, G ij) mechanical properties. The simulations are designed by applying a force equal to the force achieved in correspondence of the experimental yield point of the mechanical test. The three different materials have been modeled and evaluated under same mechanical conditions. Finally, two different reinforced materials have been simulated. Properties Matrix C.F. Young Poisson ratio Shear [GPa] [GPa] [GPa] [GPa] Yield [MPa] [MPa] 5. Experimental results The Young modules measured by experimental tests are shown in Table 1 for the three directions. The Poisson ratios are approximated by Eq. (4), with the strains at 10 MPa (ε 10.i ) and 15 MPa (ε 15.i ): ʋ xy = ε x ε y = (ε 15.x ε 10.x ) (ε 15.y ε 10.y ) (4) The method provides us only with the ʋxy Poisson ratio, hence we have supposed the same value in all the directions. The shear is computes by Eq. (2), using an estimated Poisson ratio. 6. Computational results Using the values of Table 1, the computational result for the isotropic material is quite different from the experimental value of the yield, which is MPa.
4 Then, by modifying the Poisson ratio until the value of and using the same values of E and G of Table 1, the simulation results performed better with a relative error of 3%, approximately. Table 3 gives the FEM results, the experimental stress at the yield point and the relative error for the isotropic model with ʋij = Table 3: Experimental and computational results for the isotropic material. FEM [MPa] Yield [MPa] Relative error % Figure 5 shows the von Mises stress (44.3 MPa) generated under forces at the yield stress of the material. Figure 6. FEM results for the orthotropic material. Moreover, two different reinforced materials with 17% and 47% volume of fiber have been simulated, using the previous computational model for an orthotropic material. Table 5 presents the simulation results for these reinforced materials. The von Mises stresses are plotted in Fig. 7 and Fig. 8, for the 17% volume of fiber and 47% volume of fiber, respectively. Table 5: Orthotropic model simulation results. Material (volume of fiber, %) FEM [MPa] Yield [MPa] Relative error % % Figure 5. FEM results for the isotropic material. The orthotropic material has been evaluated using the E ij and G ij of Table 1 and the Poisson ratio ʋij = The FEM results are tabulated in Table 4, while Fig. 6 plot the Von Misses stress of compression. Table 4: Results for the orthotropic model (z direction) of the 30% C.F. reinforced material. FEM [MPa] Yield [MPa] Relative error % Figure 7. FEM results for the orthotropic material, 17% reinforced volume.
5 Figure 8. FEM results for the orthotropic material, 47% reinforced volume. 7. Analysis of results and conclusions. To improve the simulation results we have had to reduce the analytical Poisson ratio to a value of 0.025, obtaining a final relative error of 3.09%, approximately. The computational results for the orthotropic model of a 3D printed reinforced material give a relative error of 16.4%. However, the reinforced polymer present several factors affecting its mechanical behavior, for example the distance between extruded filaments, width, filament pattern, layer thickness, etc. (DomingoEspin et al., 2015). Therefore, we consider that for this complex material, the previous error gives an acceptable simulation concerning the mechanical performance of a 3D printed reinforced material. Further simulations for a prototype pylon have been developed, showing that the prototype exceed the yield point (42.03 MPa) of material, needing a redesign or a topology optimization of part, as the Von Misses stresses of Fig. 9 show. The simulation of fiber reinforced materials is a challenging task. The isotropic model presented a lower error, however the orthotropic model is a better method for analyzing the mechanical performance of reinforced materials. References DomingoEspin, M. PoigoriolForcada, J. M. & GarciaGranada, A. A. Mechanical property characterization and simulation of fused deposition modeling Polycarbonate parts. Materials & Design, 83, , (2015). Góski, F. Kuczko, W. et al. Computation of Mechanical Properties of Parts Manufactured by Fused Deposition Modeling Using Finite Element Method. 10 th International Conference on Soft Figure 9. FEM results for the heel strike of a pylon prototype, using orthotropic model material, 30% reinforced volume. Computing Models in Industrial and Environmental Applications, Advances in Intelligent Systems and Computing Poland, (2015). Mallick, P. FiberReinforced Composites: Materials, Manufacturing and Design. Florida, United State: CRC Press, (2008). Sayre, R. A Comparative Finite Element Stress Analysis of Isotopic and Fusion Deposited 3D Printed Polymer. Rensselaer Polytechnic Institute, Connecticut, United State, (2014). Sutradhar, A. Park, J. Carrau, D. & Miller, M. Experimental Validation of 3D Printed Patient Specific Implants using Digital Imagen Correlation and Finite Element Analysis. Computers in Biology and Medicine 52, 817, (2014). Wu, W. Geng, P. Li, G. Zhao, D. Zang, H. Zhao, J. Influence of Layer Thickness and Raster Angle on Mechanical Properties of 3DPrinted PEEK and a Comparative Mechanical Study between PEEK and ABS. Materials Journal. 8. pp , (2015). Acknowledgements Special thanks to the Laboratory of Applied Ergonomics of Costa Rica Institute of Technology for the material supplied, and to Eng. Miguel Araya for the designs supported. Also, the financial aid of the Postgraduate Direction is very acknowledged.
Finite Element Modeling of an Aluminum Tricycle Frame
Finite Element Modeling of an Aluminum Tricycle Frame A. Rodríguez, B. Chiné*, and J. A. Ramírez Costa Rica Institute of Technology, School of Materials Science and Engineering, Cartago, Costa Rica *Corresponding
More informationComposites Design and Analysis. Stress Strain Relationship
Composites Design and Analysis Stress Strain Relationship Composite design and analysis Laminate Theory Manufacturing Methods Materials Composite Materials Design / Analysis Engineer Design Guidelines
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More information3D and Planar Constitutive Relations
3D and Planar Constitutive Relations A School on Mechanics of Fibre Reinforced Polymer Composites Knowledge Incubation for TEQIP Indian Institute of Technology Kanpur PM Mohite Department of Aerospace
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationNumerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints
THEORETICAL & APPLIED MECHANICS LETTERS 1, 041005 (2011) Numerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints M. R. Khoshravan,
More informationMATERIAL ELASTIC ANISOTROPIC command
MATERIAL ELASTIC ANISOTROPIC command.. Synopsis The MATERIAL ELASTIC ANISOTROPIC command is used to specify the parameters associated with an anisotropic linear elastic material idealization. Syntax The
More informationELASTICITY (MDM 10203)
LASTICITY (MDM 10203) Lecture Module 5: 3D Constitutive Relations Dr. Waluyo Adi Siswanto University Tun Hussein Onn Malaysia Generalised Hooke's Law In one dimensional system: = (basic Hooke's law) Considering
More informationBuckling Behavior of 3D Randomly Oriented CNT Reinforced Nanocomposite Plate
Buckling Behavior of 3D Randomly Oriented CNT Reinforced Nanocomposite Plate Outline Introduction Representative Volume Element (RVE) Periodic Boundary Conditions on RVE Homogenization Method Analytical
More information2 To whom all correspondences should be addressed:
Composite Modeling and Analysis of FDM Prototypes for Design and Fabrication of Functionally Graded Parts Longmei Li, Q. Sun, C. Bellehumeur 1,andP.Gu 2 Department of Mechanical and Manufacturing Engineering
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationComparison of Asbuilt FEA Simulations and Experimental Results for Additively Manufactured Dogbone Geometries.
Clemson University TigerPrints All Theses Theses 52017 Comparison of Asbuilt FEA Simulations and Experimental Results for Additively Manufactured Dogbone Geometries. Prathamesh Baikerikar Clemson University,
More informationStatic and Time Dependent Failure of Fibre Reinforced Elastomeric Components. Salim Mirza Element Materials Technology Hitchin, UK
Static and Time Dependent Failure of Fibre Reinforced Elastomeric Components Salim Mirza Element Materials Technology Hitchin, UK Introduction Fibre reinforced elastomers are used in many applications,
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationUnderstand basic stressstrain response of engineering materials.
Module 3 Constitutive quations Learning Objectives Understand basic stressstrain response of engineering materials. Quantify the linear elastic stressstrain response in terms of tensorial quantities
More informationAfter lecture 16 you should be able to
Lecture 16: Design of paper and board packaging Advanced concepts: FEM, Fracture Mechanics After lecture 16 you should be able to describe the finite element method and its use for paper based industry
More informationChapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING )
Chapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING ) 5.1 DEFINITION A construction member is subjected to centric (axial) tension or compression if in any cross section the single distinct stress
More informationCrack Tip Plastic Zone under Mode I Loading and the Nonsingular T zz stress
Crack Tip Plastic Zone under Mode Loading and the Nonsingular T stress Yu.G. Matvienko Mechanical Engineering Research nstitute of the Russian Academy of Sciences Email: ygmatvienko@gmail.com Abstract:
More informationOPTIMAL DESIGN OF COMPOSITE INSERTS FOR A HYBRID ULTRACENTRIFUGE ROTOR
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS OPTIMAL DESIGN OF COMPOSITE INSERTS Hak Gu Lee 1*, Jisang Park 1, Ji Hoon Kim 1 1 Composite Materials Group, KIMS, Changwon, Korea * Corresponding
More informationMECHANICS OF MATERIALS. EQUATIONS AND THEOREMS
1 MECHANICS OF MATERIALS. EQUATIONS AND THEOREMS Version 20110114 Stress tensor Definition of traction vector (1) Cauchy theorem (2) Equilibrium (3) Invariants (4) (5) (6) or, written in terms of principal
More informationLoad Cell Design Using COMSOL Multiphysics
Load Cell Design Using COMSOL Multiphysics Andrei Marchidan, Tarah N. Sullivan and Joseph L. Palladino Department of Engineering, Trinity College, Hartford, CT 06106, USA joseph.palladino@trincoll.edu
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationMATERIAL MECHANICS, SE2126 COMPUTER LAB 4 MICRO MECHANICS. E E v E E E E E v E E + + = m f f. f f
MATRIAL MCHANICS, S226 COMPUTR LAB 4 MICRO MCHANICS 2 2 2 f m f f m T m f m f f m v v + + = + PART A SPHRICAL PARTICL INCLUSION Consider a solid granular material, a so called particle composite, shown
More informationElastic parameters prediction under dynamic loading based on the. unit cell of composites considering end constraint effect
Elastic parameters prediction under dynamic loading based on the unit cell of composites considering end constraint effect Wang Meng 1,, Fei Qingguo 1,, Zhang Peiwei 1, (1. Institute of Aerospace Machinery
More informationMicromeso draping modelling of noncrimp fabrics
Micromeso draping modelling of noncrimp fabrics Oleksandr Vorobiov 1, Dr. Th. Bischoff 1, Dr. A. Tulke 1 1 FTA Forschungsgesellschaft für Textiltechnik mbh 1 Introduction Noncrimp fabrics (NCFs) are
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationEVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS EVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS T. Kurashiki 1 *, Y. Matsushima 1, Y. Nakayasu
More informationFiniteElement Analysis of Stress Concentration in ASTM D 638 Tension Specimens
Monika G. Garrell, 1 Albert J. Shih, 2 Edgar LaraCurzio, 3 and Ronald O. Scattergood 4 Journal of Testing and Evaluation, Vol. 31, No. 1 Paper ID JTE11402_311 Available online at: www.astm.org FiniteElement
More informationScienceDirect. Unit cell model of woven fabric textile composite for multiscale analysis. Anurag Dixit a *,Harlal Singh Mali b, R.K.
Available online at www.sciencedirect.com ScienceDirect Procedia Engineering 68 ( 2013 ) 352 358 The Malaysian International Tribology Conference 2013 (MITC2013) Unit cell model of woven fabric textile
More information2. Mechanics of Materials: Strain. 3. Hookes's Law
Mechanics of Materials Course: WB3413, Dredging Processes 1 Fundamental Theory Required for Sand, Clay and Rock Cutting 1. Mechanics of Materials: Stress 1. Introduction 2. Plane Stress and Coordinate
More informationDetermination of the Shear Buckling Load of a Large Polymer Composite ISection Using Strain and Displacement Sensors
Sensors 2012, 12, 1602416036; doi:10.3390/s121216024 Article OPEN ACCESS sensors ISSN 14248220 www.mdpi.com/journal/sensors Determination of the Shear Buckling Load of a Large Polymer Composite ISection
More informationCIV E 205 Mechanics of Solids II. Course Notes
University of Waterloo Department of Civil Engineering CIV E 205 Mechanics of Solids II Instructor: Tarek Hegazi Room: CPH 2373 G, Ext. 2174 Email: tarek@uwaterloo.ca Course Web: www.civil.uwaterloo.ca/tarek/hegazy205.html
More informationStrain Transformation equations
Strain Transformation equations R. Chandramouli Associate DeanResearch SASTRA University, Thanjavur613 401 Joint Initiative of IITs and IISc Funded by MHRD Page 1 of 8 Table of Contents 1. Stress transformation
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationA PAPER ON DESIGN AND ANALYSIS OF PRESSURE VESSEL
A PAPER ON DESIGN AND ANALYSIS OF PRESSURE VESSEL P.Palanivelu 1, R.Siva Prasad 2, 1 PG Scholar, Department of Mechanical Engineering, Gojan School of Business and Technology, Redhills, Chennai, India.
More informationInfluence of the filament winding process variables on the mechanical behavior of a composite pressure vessel
Influence of the filament winding process variables on the mechanical behavior of a composite pressure vessel G. Vargas 1 & A. Miravete 2 1 Universidad Pontificia Bolivariana, Facultad de Ingeniería Mecánica,
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationFinal Analysis Report MIE 313 Design of Mechanical Components
Final Analysis Report MIE 313 Design of Mechanical Components Juliana Amado Charlene Nestor Peter Walsh Table of Contents Abstract:...iii Introduction:... 4 Procedure:... 5 Results:... 6 Reliability:...
More informationSimulation of the Influence of Manufacturing Quality on Thermomechanical Stress of Microvias
As originally published in the IPC APEX EXPO Conference Proceedings. Simulation of the Influence of Manufacturing Quality on Thermomechanical Stress of Microvias Yan Ning, Michael H. Azarian, and Michael
More informationPLAIN WEAVE REINFORCEMENT IN C/C COMPOSITES VISUALISED IN 3D FOR ELASTIC PARAMETRES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS PLAIN WEAVE REINFORCEMENT IN C/C COMPOSITES VISUALISED IN 3D FOR ELASTIC PARAMETRES P. Tesinova Technical University of Liberec, Faculty of Textile
More informationPlane Strain Test for Metal Sheet Characterization
Plane Strain Test for Metal Sheet Characterization Paulo Flores 1, Felix Bonnet 2 and AnneMarie Habraken 3 1 DIM, University of Concepción, Edmundo Larenas 270, Concepción, Chile 2 ENS  Cachan, Avenue
More informationResearch on Crowning Profile to Obtain Maximum Load Carrying Capacity for Roller Bearings
Research on Crowning Profile to Obtain Maximum Load Carrying Capacity for Roller Bearings S. KAMAMOTO * K. FUJIMOTO ** T. YAMAMOTO *** * Mechatronic Systems Research & Development Department, Research
More informationAvailable online at ScienceDirect. 20th European Conference on Fracture (ECF20) Yu.G. Matvienko*
Available online at www.sciencedirect.com ScienceDirect Procedia Materials Science 3 ( 014 ) 141 146 0th European Conference on Fracture (ECF0) The Effect of the nonsingular Tstress components on crack
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationChapter 3. Load and Stress Analysis
Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3
More informationCONSTITUTIVE RELATIONS FOR LINEAR ELASTIC SOLIDS
Chapter 9 CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS Figure 9.1: Hooke memorial window, St. Helen s, Bishopsgate, City of London 211 212 CHAPTR 9. CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS 9.1 Mechanical
More informationIdentification of the plastic zone using digital image correlation
M. Rossi et alii, Frattura ed Integrità Strutturale, 3 (4) 55557; DOI:.3/IGFESIS.3.66 Focussed on: Fracture and Structural Integrity related Issues Identification of the plastic zone using digital image
More informationEFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES
EFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES OF WOOD OR PLYWOOD CONSIDERED AS ORTHOTROPIC MATERIALS Information Revied and Reaffirmed March 1956 No. 1510 EFFECT OF ELLIPTIC
More informationBone Tissue Mechanics
Bone Tissue Mechanics João Folgado Paulo R. Fernandes Instituto Superior Técnico, 2016 PART 1 and 2 Introduction The objective of this course is to study basic concepts on hard tissue mechanics. Hard tissue
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationExperimental Study and Numerical Simulation on Steel Plate Girders With Deep Section
6 th International Conference on Advances in Experimental Structural Engineering 11 th International Workshop on Advanced Smart Materials and Smart Structures Technology August 12, 2015, University of
More informationShear stresses around circular cylindrical openings
Shear stresses around circular cylindrical openings P.C.J. Hoogenboom 1, C. van Weelden 1, C.B.M. Blom 1, 1 Delft University of Technology, the Netherlands Gemeentewerken Rotterdam, the Netherlands In
More informationTHE MECHANICAL BEHAVIOR OF ORIENTED 3D FIBER STRUCTURES
Lappeenranta University of Technology School of Engineering Science Degree Program in Computational Engineering and Technical Physics Master s Thesis Alla Kliuzheva THE MECHANICAL BEHAVIOR OF ORIENTED
More informationPlane and axisymmetric models in Mentat & MARC. Tutorial with some Background
Plane and axisymmetric models in Mentat & MARC Tutorial with some Background Eindhoven University of Technology Department of Mechanical Engineering Piet J.G. Schreurs Lambèrt C.A. van Breemen March 6,
More informationStress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole
Stress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole Dheeraj Gunwant, J. P. Singh mailto.dheerajgunwant@gmail.com, jitenderpal2007@gmail.com, AIT, Rampur Abstract A static
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationUNIT I SIMPLE STRESSES AND STRAINS
Subject with Code : SM1(15A01303) Year & Sem: IIB.Tech & ISem SIDDHARTH GROUP OF INSTITUTIONS :: PUTTUR Siddharth Nagar, Narayanavanam Road 517583 QUESTION BANK (DESCRIPTIVE) UNIT I SIMPLE STRESSES
More informationCOMPRESSION AND BENDING STIFFNESS OF FIBERREINFORCED ELASTOMERIC BEARINGS. Abstract. Introduction
COMPRESSION AND BENDING STIFFNESS OF FIBERREINFORCED ELASTOMERIC BEARINGS HsiangChuan Tsai, National Taiwan University of Science and Technology, Taipei, Taiwan James M. Kelly, University of California,
More informationExperimental and theoretical characterization of Li 2 TiO 3 and Li 4 SiO 4 pebbles
Experimental and theoretical characterization of Li 2 TiO 3 and Li 4 SiO 4 s D. Aquaro 1 N. Zaccari ABSTRACT Dipartimento di Ingegneria Meccanica Nucleare e della Produzione University of Pisa (Italy)
More informationComputational models of diamond anvil cell compression
UDC 519.6 Computational models of diamond anvil cell compression A. I. Kondrat yev Independent Researcher, 5944 St. Alban Road, Pensacola, Florida 32503, USA Abstract. Diamond anvil cells (DAC) are extensively
More informationAnisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA
Anisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA Alexandre Hatt 1 1 Faurecia Automotive Seating, Simplified Limited Liability Company 1 Abstract / Summary Polymer thermoplastics
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More information9 Strength Theories of Lamina
9 trength Theories of Lamina 9 TRENGTH O ORTHOTROPIC LAMINA or isotropic materials the simplest method to predict failure is to compare the applied stresses to the strengths or some other allowable stresses.
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationAssisted by Advanced FiniteElement Simulations
Presented at the COMSOL Conference 2009 Milan COMSOL 2009, Milan, October 2009 Magnetic Fields in Hochfeld Magnetlabor Dresden Science and Medicine Assisted by Advanced FiniteElement Simulations HochfeldMagnetlabor
More informationModeling of FiberReinforced Membrane Materials Daniel Balzani. (Acknowledgement: Anna Zahn) Tasks Week 2 Winter term 2014
Institute of echanics and Shell Structures Faculty Civil Engineering Chair of echanics odeling of FiberReinforced embrane aterials OOC@TU9 Daniel Balani (Acknowledgement: Anna Zahn Tasks Week 2 Winter
More informationMechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationDesign of a fastener based on negative Poisson's ratio foam adapted from
1 Design of a fastener based on negative Poisson's ratio foam adapted from Choi, J. B. and Lakes, R. S., "Design of a fastener based on negative Poisson's ratio foam", Cellular Polymers, 10, 205212 (1991).
More informationTorsional Shear Strength and Size Effect in Structural Composite Lumber
University of Massachusetts Amherst ScholarWorks@UMass Amherst Masters Theses 1911  February 2014 2012 Torsional Shear Strength and Size Effect in Structural Composite Lumber Zhuo Yang University of Massachusetts
More informationNonlinear Finite Element Modeling of Nano Indentation Group Members: Shuaifang Zhang, Kangning Su. ME 563: Nonlinear Finite Element Analysis.
ME 563: Nonlinear Finite Element Analysis Spring 2016 Nonlinear Finite Element Modeling of Nano Indentation Group Members: Shuaifang Zhang, Kangning Su Department of Mechanical and Nuclear Engineering,
More informationBasic Concepts of Strain and Tilt. Evelyn Roeloffs, USGS June 2008
Basic Concepts of Strain and Tilt Evelyn Roeloffs, USGS June 2008 1 Coordinates Righthanded coordinate system, with positions along the three axes specified by x,y,z. x,y will usually be horizontal, and
More information3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture,
3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture, 09.21.07 1. In the beam considered in PS1, steel beams carried the distributed weight of the rooms above. To reduce stress on the beam, it
More informationValidation of COMSOL Based Performance Predictions of Bi2212 Round Wire Prototype Coils
Validation of COMSOL Based Performance Predictions of Bi2212 Round Wire Prototype Coils Ernesto S. Bosque U.P. Trociewitz Y.Kim, D.K. Hilton, C.L. English, D.S. Davis, G. Miller, D. Larbalestier Bi2212
More informationCHAPTER 3 THE EFFECTS OF FORCES ON MATERIALS
CHAPTER THE EFFECTS OF FORCES ON MATERIALS EXERCISE 1, Page 50 1. A rectangular bar having a crosssectional area of 80 mm has a tensile force of 0 kn applied to it. Determine the stress in the bar. Stress
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More information6. Bending CHAPTER OBJECTIVES
CHAPTER OBJECTIVES Determine stress in members caused by bending Discuss how to establish shear and moment diagrams for a beam or shaft Determine largest shear and moment in a member, and specify where
More informationSymmetric Bending of Beams
Symmetric Bending of Beams beam is any long structural member on which loads act perpendicular to the longitudinal axis. Learning objectives Understand the theory, its limitations and its applications
More informationFINITE ELEMENT ANALYSIS OF THE ELASTIC CONSTITUTIVE BEHAVIOR OF A 2.5D INTERLOCK COMPOSITE
FINITE ELEMENT ANALYSIS OF THE ELASTIC CONSTITUTIVE BEHAVIOR OF A 2.5D INTERLOCK COMPOSITE NEHME Samer *, HAGEGE Benjamin *, KAABI Abderrahmen **, BENZEGGAGH Malk * * Université de Technologie de Compiègne,
More informationANSYS Mechanical Basic Structural Nonlinearities
Lecture 4 Rate Independent Plasticity ANSYS Mechanical Basic Structural Nonlinearities 1 Chapter Overview The following will be covered in this Chapter: A. Background Elasticity/Plasticity B. Yield Criteria
More informationJeff Brown Hope College, Department of Engineering, 27 Graves Pl., Holland, Michigan, USA UNESCO EOLSS
MECHANICS OF MATERIALS Jeff Brown Hope College, Department of Engineering, 27 Graves Pl., Holland, Michigan, USA Keywords: Solid mechanics, stress, strain, yield strength Contents 1. Introduction 2. Stress
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationDetermination of Poisson s Ratio of Rock Material by Changing Axial Stress and Unloading Lateral Stress Test
Rock Mech Rock Eng DOI 10.1007/s0060301405869 TECHNICAL NOTE Determination of Poisson s Ratio of Rock Material by Changing Axial Stress and Unloading Lateral Stress Test Xiangtao Xu Runqiu Huang Hua
More informationComposite Laminate Modeling
omposite Laminate Modeling White Paper for Femap and NX Nastran Users Venkata Bheemreddy, Ph.D., Senior Staff Mechanical Engineer Adrian Jensen, PE, Senior Staff Mechanical Engineer WHAT THIS WHITE PAPER
More informationSupplementary Information to the article entitled: Internally Architectured Materials with Directionally Asymmetric Friction
Supplementary Information to the article entitled: Internally Architectured Materials with Directionally Asymmetric Friction Ehsan Bafekrpour 1,2, Arcady Dyskin 3, Elena Pasternak 4, Andrey Molotnikov
More informationDruckerPrager yield criterion application to study the behavior of CFRP confined concrete under compression
XXXVII IAHS World ongress on Housing October 6 9, 00, Santander, Spain DruckerPrager yield criterion application to study the behavior of FRP confined concrete under compression Salvador Ivorra, Ramón
More informationCOURSE STE6289 Modern Materials and Computations (Moderne materialer og beregninger 7.5 stp.)
Narvik University College (Høgskolen i Narvik) EXAMINATION TASK COURSE STE6289 Modern Materials and Computations (Moderne materialer og beregninger 7.5 stp.) CLASS: Master students in Engineering Design
More informationAn Integrated Thermomechanical Method for Modeling Fiber Reinforced Polymer Composite Structures in Fire. Ziqing Yu¹ and Aixi Zhou²
An Integrated Thermomechanical Method for Modeling Fiber Reinforced Polymer Composite Structures in Fire Ziqing Yu¹ and Aixi Zhou² ¹Department of Engineering Technology, University of North Carolina at
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 15 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationBALLISTIC IMPACT MODELING OF COMPOSITE MATERIALS
7 th International LSDYNA Users Conference Penetration/Explosive BALLISTIC IMPACT MODELING OF COMPOSITE MATERIALS ChianFong Yen Materials Sciences Corporation 5 Office Center Drive Fort Washington, PA
More information3D Compression Molding
Autodesk Simulation Moldflow Insight 2014 3D Compression Molding Executive summary In this work, the simulation results from a program developed for the threedimensional analysis of compression molding
More informationASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE MATERIAL
5 th International Conference Advanced Composite Materials Engineering COMAT 2014 1617 October 2014, Braşov, Romania ASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE
More informationTensor Visualization. CSC 7443: Scientific Information Visualization
Tensor Visualization Tensor data A tensor is a multivariate quantity Scalar is a tensor of rank zero s = s(x,y,z) Vector is a tensor of rank one v = (v x,v y,v z ) For a symmetric tensor of rank 2, its
More informationA Finite Element Model for Numerical Analysis of Sintering
A Finite Element Model for Numerical Analysis of Sintering DANIELA CÂRSTEA HighSchool Group of Railways, Craiova ION CÂRSTEA Department of Computer Engineering and Communication University of Craiova
More information